# Temperature dependence of electronic behaviors in quantum dimension junctionless thin-film transistor

- Ya-Chi Cheng
^{1}, - Hung-Bin Chen
^{1, 2}, - Ming-Hung Han
^{2}, - Nan-Heng Lu
^{1}, - Jun-Ji Su
^{1}, - Chi-Shen Shao
^{2}and - Yung-Chun Wu
^{1}Email author

**9**:392

**DOI: **10.1186/1556-276X-9-392

© Cheng et al.; licensee Springer. 2014

**Received: **8 April 2014

**Accepted: **9 July 2014

**Published: **13 August 2014

## Abstract

The high temperature dependence of junctionless (JL) gate-all-around (GAA) poly-Si thin-film transistors (TFTs) with 2-nm-thick nanosheet channel is compared with that of JL planar TFTs. The variation of SS with temperature for JL GAA TFTs is close to the theoretical value (0.2 mV/dec/K), owing to the oxidation process to form a 2-nm-thick channel. The bandgap of 1.35 eV in JL GAA TFTs by fitting experimental data exhibits the quantum confinement effect, indicating greater suppression of I_{off} than that in JL planar TFTs. The measured $\frac{\partial {V}_{\mathit{th}}}{\partial T}$ of −1.34 mV/°C in JL GAA nanosheet TFTs has smaller temperature dependence than that of −5.01 mV/°C in JL planar TFTs.

### Keywords

Junctionless Nanowire Thin-film transistor (TFTs) Gate-all-around (GAA) Quantum confinement effect## Background

The junctionless nanowire transistor (JNT), which contains a single doping species at the same level in its source, drain, and channel, has been recently investigated [1–6]. The junctionless (JL) device is basically a gated resistor, in which the advantages of junctionless devices include (1) avoidance of the use of an ultra shallow source/drain junction, which greatly simplifies the process flow; (2) low thermal budgets owing to implant activation anneal after gate stack formation is eliminated, and (3) the current transport is in the bulk of the semiconductor, which reduces the impact of imperfect semiconductor/insulator interfaces. As is widely recognized, the temperature dependence of threshold voltage (*V*_{th}) is a parameter when integrated circuits often operate at an elevated temperature owing to heat generation. This effect, accompanied with the degradation of subthreshold swing (SS) with temperature, causes the fatal logic errors, leakage current, and excessive power dissipation. Despite a previous work that characterized JNTs at high temperatures [7], there is no information regarding the JL thin-film transistor (TFT) at a high temperature yet. Hence, this letter presents a high-temperature operation of JL TFTs with a gate-all-around structure (GAA) for an ultra-thin channel. The JL TFT with a planar structure functions as the control device. The drain current (*I*_{d}), SS, off-leakage current (*I*_{off}), and *V*_{th} are also evaluated for fabricated devices. The JL GAA TFTs with a small variation in temperature performances along with simple fabrication are highly promising for future system-on-panel (SOP) and system-on-chip (SOC) applications.

## Methods

The process for producing 2-nm-thick poly-Si nanosheet channel was fabricated by initially growing a 400-nm-thick thermal silicon dioxide layer on 6-inch silicon wafers. Subsequently, a 40-nm-thick undoped amorphous silicon (a-Si) layer was deposited by low-pressure chemical vapor deposition (LPCVD) at 550°C. Then, the a-Si layer was solid-phase recrystallized (SPC) and formed large grain sizes as a channel layer at 600°C for 24 h in nitrogen ambient. The channel layer was implanted with 16-keV phosphorous ions at a dose of 1 × 10^{14} cm^{−2}, followed by furnace annealing at 600°C for 4 h. Subsequently, we performed a wet trimming process with a dilute HF chemical solution at room temperature and shrink down channel thickness to be around 28 nm. The active layers, serving as channel, were defined by e-beam lithography and then mesa-etched by time-controlled wet etching of the buried oxide to release the poly-Si bodies. Subsequently, a 13-nm-thick dry oxide, consuming around 13-nm-thick poly-Si on both side of channel to form 2-nm-thick channel, and 6-nm-thick nitride by LPCVD were deposited as the gate oxide layer. The 250-nm-thick in-situ doped n + poly-silicon was deposited as a gate electrode, and patterned by e-beam and reactive ion etching. Finally, passivation layer and metallization was performed. The JL planar TFT serves as a control with single gate structure.

## Results and discussion

*I*

_{d}as a function of gate bias (

*V*

_{g}) at various temperatures ranging from 25°C to 200°C at

*V*

_{d}= 0.5 V for (a) JL planar TFTs with channel length (

*L*

_{g}) of 1 μm, (b) JL GAA TFTs with

*L*

_{g}= 1 μm, and (c) JL GAA TFTs with

*L*

_{g}= 60 nm. This figure reveals that

*V*

_{th}decreases and the SS increases in all devices when increasing the temperature. Figure 3 presents the measured SS and

*I*

_{off}as a function of temperature at

*V*

_{d}= 0.5 V, as extracted from the

*I*

_{d}-

*V*

_{g}curves in Figure 2. In Figure 3a, the JL GAA TFTs have a small SS variation with temperature than JL planar TFTs. Furthermore, the SS can be expressed as follows [8]:

*C*

_{ox}is the gate oxide capacitance per unit area,

*N*

_{T}is the trap states, and

*t*

_{Si}is the thickness of the poly-Si layer. Therefore, the decline in SS of JL GAA TFTs is due to a decreasing

*t*

_{Si}and the formation of a crystal-like channel by oxidation. The variation of the SS with temperature $\left(\frac{\partial \mathrm{SS}}{\partial T}\right)$ for JL GAA TFTs is 0.25 mV/dec/K, which is slightly larger than the theoretical value of 0.2 mV/dec/K. The results represent the second term of Equation 1 is small and insensitive to temperature. According to Figure 3b,

*I*

_{off}is defined as the drain current at

*V*

_{g}= −1.9 V for JL planar TFTs and at

*V*

_{g}= −0.2 V for JL GAA TFTs, respectively. Moreover,

*I*

_{off}can be expressed as follows [9]:

*I*

_{sub}is the subthreshold current,

*I*

_{leak}is the trap-induced leakage current, and

*E*

_{g}is the bandgap. The

*E*

_{g}could be regarded as a constant value for estimation, because $\frac{\partial {E}_{g}}{\partial T}$ is known to be −0.27 meV/K [10]. Therefore, the

*E*

_{g}of JL planar and GAA TFTs, as extracted by Equation 2, is around 1.12 and 1.35 eV, respectively. Notably, quantum confinement is observed in JL GAA TFTs, resulting in band-edge shifts (Δ

*E*

_{c}) of the conduction-band and valence-band, thereby increasing the

*E*

_{g}to reduce the off-state leakage current, as shown in Figure 3c. Figure 3c illustrates the band diagram of the GAA device in off-state with discrete energy levels. The GAA device is simulated by solving 3D quantum-corrected device simulation using the commercial tool, Synopsys Sentaurus Device [11], [12] to obtain accurate numerical results for a nanometer-scale device. These simulation performances are calibrated to experimental data of

*I*

_{d}–

*V*

_{g}. The Δ

*E*

_{c}is estimated around 0.23 eV, as extracted from the experimental data in Figure 3b. The theoretical analysis derived from the solution of the Schrödinger equation for the first level in the conduction band as follows [10]:

where *m*_{e}* is the electron effective mass, *h* is Plank's constant, *T*_{ch} is the channel thickness and *W* is the channel width. The second term in Equation 3, which represents quantum confinement effect in the channel width direction, can be ignored due to *W* > > *T*_{ch}. The Δ*V*_{th} of theoretical value is 0.36 eV, which is larger than experimental value of 0.23 eV. The gap would come from the poly-Si channel material.

*V*

_{th}as a function of temperature. The

*V*

_{th}is defined as the gate voltage at

*I*

_{d}= 10

^{−9}A. The temperature coefficients of

*V*

_{th}are −1.34 and −5.01 mV/°C for GAA and planar JL TFTs, respectively. According to [13], the variation of $\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ in n-type JL devices can be expressed as follows [13]:

where *V*_{fb} is the flat-band voltage, *C*_{ox} is the gate oxide capacitance per unit length, *A* is the device cross-sectional area and *P* is the gate perimeter. The first term in the right side of Equation 4 is depended on the flat-band voltage variation with temperature. For *N*_{D} = 1 × 10^{19} cm^{−3}, the value of $\frac{\partial {V}_{\mathrm{fb}}}{\partial T}$ is approach to −0.49 mV/°C as the devices in [13], which has a P^{+} polycrystalline silicon gate and the same doping concentration. The second term represents the effect of incomplete ionization. The doped impurities are almost completely ionized at those temperatures higher than room temperature. Thus, the doping concentration variation with the temperature $\left(\frac{\partial {N}_{D}}{\partial T}\right)$ has a slight dependence on temperature. The third term, depending on the electron effective mass, also has a smaller dependence on *T* than the other terms. The theoretical value of $\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ is about −0.49 mV/°C; although the $\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ of −1.34 mV/°C in JL GAA TFTs is larger than theoretical value, but is comparable with current SOI-based JNT ($\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ approximately −1.63 mV/°C) [7] due to the use of the multi-gate structure and formation of a crystal-like nanosheet channel with fewer traps by oxidation process. Therefore, JL TFTs with the GAA structure and ultra-thin channel shows an excellent immunity to the temperature dependence on *V*_{th} and competes with SOI-based JNT. Figure 4b presents the measured on-current (*I*_{on}) as a function of temperature. The *I*_{on} is defined as the drain current at *V*_{g} = 3 V for JL planar TFTs and at *V*_{g} = 6 V for JL GAA TFTs. The JL GAA TFTs show a slightly better *I*_{on} variation with temperature than the planar ones, possibly owing to a smaller $\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ in JL GAA TFTs.

## Conclusion

This work has presented a high-temperature operation of JL TFTs. The high temperature dependence of JL GAA and planar TFTs is also studied. The variation of parameters such as *V*_{th}, *I*_{on}, SS, and *I*_{off} are analyzed as well. The variation of the SS with temperature for JL GAA TFTs is close to the ideal value (0.2 mV/dec/K) owing to the ability of the oxidation process to form a nanosheet channel and crystal-like channel. Additionally, *I*_{off} is negligibly small for JL GAA TFTs, owing to quantum confinement effect; its *E*_{g} of 1.35 eV is also extracted. The JL GAA TFTs have a smaller $\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ than that of JL planar TFTs owing to the GAA structure and ultra-thin channel. Moreover, the measured $\frac{\partial {V}_{\mathrm{th}}}{\partial T}$ of JL GAA TFTs competes with that of SOI-based JNTs. Therefore, the JL GAA TFTs with a slight variation in temperature performances along with simple fabrication are highly promising for future SOP and system-on-chip SOC applications.

## Declarations

### Acknowledgements

The authors would like to acknowledge the National Science Council of Taiwan for supporting this research under Contract No. MOST 103-2221-E-007 -114 -MY3. The National Nano Device Laboratories is greatly appreciated for its technical support.

## Authors’ Affiliations

## References

- Lee CW, Afzalian A, Akhavan ND, Yan R, Ferain I, Colinge JP: Junctionless multigate field-effect transistor.
*Appl Phys Lett*2009, 94: 053511. 10.1063/1.3079411View Article - Colinge JP, Lee CW, Afzalian A, Akhavan ND, Yan R, Ferain I, Razavi P, O’Neil B, Blake A, White M, Kelleher AM, McCarthy B, Murphy R: Nanowire transistors without junctions.
*Nat Nanotechnol*2010, 5: 225. 10.1038/nnano.2010.15View Article - Colinge JP, Lee CW, Ferain I, Akhavan ND, Yan R, Razavi P, Yu R, Nazarov AN, Doria RT: Reduced electric field in junctionless transistors.
*Appl Phys Lett*2010, 96: 073510. 10.1063/1.3299014View Article - Lin HD, Lin CI, Huang TY: Characteristics of n-Type Junctionless Poly-Si Thin-Film Transistors With an Ultrathin Channel.
*IEEE Electron Device Lett*2012, 33: 53.View Article - Su CJ, Tsai TI, Liou YL, Lin ZM, Lin HC, Chao TS: Gate-all-around junctionless transistors with heavily doped polysilicon nanowire channels.
*IEEE Electron Device Lett*2011, 32: 521.View Article - Rios R, Cappellani A, Armstrong M, Budrevich A, Gomez H, Pai R, Rahhal-orabi N, Kuhn K: Comparison of Junctionless and conventional trigate transistors with Lg down to 26 nm.
*IEEE Electron Device Lett*2011, 32: 1170.View Article - Lee CW, Borne A, Ferain I, Afzalian A, Yan R, Akhavan ND, Razavi P, Colinge JP: High-temperature performance of silicon junctionless MOSFETs.
*IEEE Electron Device*2010, 57: 620.View Article - Dimitriadis CA: Gate bias instability in hydrogenated polycrystalline silicon thin film transistors.
*J Appl Phys*2000, 88: 3624. 10.1063/1.1289525View Article - Guo X, Ishii T, Silva SRP: Improving switching performance of thin-film transistors in disordered silicon.
*IEEE Electron Device Lett*2008, 29: 588.View Article - Sze SM, Ng K:
*Physics of Semiconductor Devices*. 3rd edition. New York: Wiley; 2007. - Synopsys, Inc:
*Sentaurus Device User Guide*. Mountain View: Version I-2013.12; 2013. - Ancona MG, Iafrate GJ: Quantum correction to the equation of state of an electron gas in a semiconductor.
*Phys Rev B*1989, 39: 9536. 10.1103/PhysRevB.39.9536View Article - Trevisoli RD, Doria RT, de Souza M, Pavanello MA: Threshold voltage in junctionless nanowire transistors.
*Semiconductor Sci Technol*2011, 26: 1.View Article

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.